O R I G I N A L

### Strength grading of Norway spruce structural timber:

### revisiting property relationships used in EN 338

### classification system

Rene´ SteigerÆ Martin Arnold

Received: 21 December 2007 / Published online: 30 September 2008 Springer-Verlag 2008

Abstract Solid timber for structural applications has to be strength graded prior to its use. In order to remain economic the grading process usually focuses on the most important physical and mechanical properties: density, modulus of elasticity (MOE) and bending strength. Based on respective limits given in standards, the timber is assigned to strength classes. Additional mechanical properties such as tensile and compression strength parallel to the grain are derived from the basic property values by empirical relationships. The objective of this study was to review some of these property relationships based on recently compiled large data sets as a contribution for a future revision of the grading standards. Based on mechanical tests of Norway spruce structural timber with different cross-sections, the following characteristic values and property relationships were evaluated: (a) strength and MOE in bending, (b) in-grade characteristic values of bending strength, bending MOE and density, (c) relationship of characteristic values of tension and compression strength parallel to the grain with respect to the corresponding characteristic value of bending strength, (d) ratio of fifth percentiles and mean values of density and MOE, as well as (e) the ratio of MOE in bending, tension and compression. Mechanical tests were accompanied by measurements of density and ultrasonic wave speed. Resulting dynamic MOE was partly used as an indicator of timber quality.

R. Steiger (*&) M. Arnold*

Empa, Swiss Federal Laboratories for Materials Testing and Research, Wood Laboratory, U¨ berlandstrasse 129, 8600 Du¨bendorf, Switzerland e-mail: rene.steiger@empa.ch

M. Arnold

e-mail: martin.arnold@empa.ch DOI 10.1007/s00226-008-0221-6

Introduction

Solid timber for structural applications has to be strength graded prior to its use. Grading standards provide strength class systems to assign timber samples to specific strength classes. In order to remain simple and economic the grading process usually focuses on the most important physical and mechanical properties: density, modulus of elasticity parallel to the grain (MOE) and bending strength (MOR). To account for the variation of mechanical properties, the classification is based on so-called characteristic values, which are fifth percentile or mean values, respectively.

In Europe, the classification of structural timber is carried out according to a set of three linked standards:

• Test methods to determine mechanical properties as well as dimensions,

moisture content (MC) and wood density of test pieces are specified in EN 408 (2003). The methods apply to rectangular and circular shapes of solid unjointed timber or finger-jointed timber and glued laminated timber with constant cross-sections. The tests have to be carried out in dried conditions (20C/65% relative humidity).

• Characteristic values of mechanical properties and density are derived from the

test data according to EN 384 (2004). The standard provides rules for sampling, analysing (e. g. calculating adjusted fifth percentiles weighted according to the number of specimens in each sample) and adjusting test values to geometrical or climatic properties differing from reference conditions given in EN 408.

• The timber is finally classified according to EN 338 (2003). This standard

defines 12 strength classes for softwoods, prefixed C: C14, C16, C18, C20, C22,

C24, C27, C30, C35, C40, C45, and C50 (Table1). The numbers represent the

characteristic bending strength fm,kfor each strength class. A specific population

can be assigned to a certain strength class if the characteristic values of density rkand bending strength fm,k(both of them are 5th-percentiles) as well as MOE

(mean value, usually derived from bending tests) match or exceed the values of the desired class. Additional mechanical properties needed for the design of timber structures are derived from these basic values by empirical relationships.

Relationship of bending strength and bending MOE

Modulus of elasticity derived from bending tests correlates well with MOR. Coefficients of correlation R up to 0.7–0.8 are reported in the literature (Glos1995). Since MOE can be derived by non-destructive tests, it is a very important parameter for machine grading. Most grading machines make use of MOE as an indicator for

timber strength (Fewell1982; Glos1995). MOE can be determined either by static

bending or dynamic methods (vibration, ultrasound) (Hearmon1966; Kollmann and

Simultaneous matching of in-grade characteristic values of MOR, mean MOE and density

In practical design of timber structures, MOR and MOE are important parameters, the latter being of even more importance since deformations of structural elements are often decisive in the course of the design process (Thelandersson1995). Compressive strength parallel to the grain as well as embedding strength has been reported to

correlate with density (Ehlbeck and Werner 1992; Fewell 1982; Gindl and

Teischinger2002; Kollmann and Coˆte´1968). Therefore, EN 338 assigns a timber

population to a strength class, if its characteristic values of bending strength and density (fifth percentiles) and its characteristic mean modulus of elasticity in bending equals or exceeds the limits for that respective strength class (Table1). Hence, it is of utmost importance that within all grades, these three basic values match as good as possible. If, for example, a specific population which fulfils the criterion for MOR and MOE has to be graded down to a lower class because the density values are not reached, it has to be questioned if density limits are set correctly.

Ratio of tensile and compression strength parallel to the grain to bending strength

Both parallel-to-the-grain tensile and compression strength are used when designing axially loaded timber members. Respective characteristic values ft,0,kand fc,0,kin EN

338 (Table1) are derived from characteristic MOR fm,k using empirical

relationships.

According to EN 384 (2004) the characteristic values of tensile strength parallel to the grain ft,0,kfor softwood species can be calculated with Eq. (1):

ft;0;k¼ 0:6 fm;k ð1Þ

This constant ratio is used in most strength class systems for structural timber

(Green and Kretschmann1990), although it was shown in several studies not to

Table 1 European strength class system for softwood species according to EN 338 (basic property values used for the classification are printed bold)

Properties (N/mm2) Strength classes C14 C16 C18 C20 C22 C24 C27 C30 C35 C40 C45 C50 Bending fm,k 14 16 18 20 22 24 27 30 35 40 45 50 Tension || ft,0,k 8 10 11 12 13 14 16 18 21 24 27 30 Compression || fc,0,k 16 17 18 19 20 21 22 23 25 26 27 29

Mean MOE || E0,mean 7,000 8,000 9,000 9,500 10,000 11,000 11,500 12,000 13,000 14,000 15,000 16,000

5th-percentile of MOE ||

E0,05 4,700 5,400 6,000 6,400 6,700 7,400 7,700 8,000 8,700 9,400 10,000 10,700

Mean density rmean 350 370 380 390 410 420 450 460 480 500 520 550

5th-percentile of density

be constant but rather to depend on timber quality. Burger and Glos (1997)

found a noticeable effect of both grading method and dimensions on the ft/fm

ratio. The ratio ft/fmrises with increasing timber quality and thus with increasing

strength. Burger and Glos (1997) reported a ft/fm ratio of 0.69 for the fifth

percentile level while the ratio on the 50th-percentile level was found to be 0.76. In the course of their discussion of timber property relationships in Eurocode 5,

Green and Kretschmann (1989) compared ultimate bending strength and tensile

strength parallel to the grain for in-grade data resulting from tests of different softwood species (Douglas fir, larch, Hemlock and Southern pine). For values of ultimate tensile strength up to 55 N/mm2 the average ratio was ft,0,k/fm,k= 0.59.

Above that limit, the ratio increased slightly. The authors, however, suggested retaining Eq. (1).

Furthermore, EN 384 gives Eq. (2) to derive the characteristic values of

compression strength parallel to the grain fc,0,k for softwood species from the

corresponding bending strength fm,k:

fc;0;k¼ 5 fm;k

0:45

ð2Þ For in-grade tested Douglas fir-larch, Hem-fir and Southern pine, Green and Kretschmann (1989) found the trend of the relationship to be virtually identical to

the data presented by Curry and Fewell (1977), which forms the basis of Eq. (2)

above. However, in earlier (Ylinen 1942) and recent (Ruli 2004) publications a

strong correlation between compression strength parallel to the grain and wood density is reported.

Ratio of fifth percentiles and mean value of density and MOE

Since density correlates well with compression strength (parallel as well as perpendicular to the grain) and embedding strength, respective characteristic values can be derived from this basic property. Strength values normally are fifth percentiles and thus these values have to be based in the fifth percentile of density. In EN 338, the in-grade characteristic value of density is derived from the grade’s mean value assuming a specific coefficient of variation (COV). The ratio of the characteristic to the mean value of density given in EN 338 varies between 0.82 and 0.85 with an average of 0.84 (Table1). This variation results from rounding. Former versions of EN 384 explicitly assumed a constant ratio of 0.84 for softwood species, which in case of a normally distributed sample is identical to a COV of 10%. Green

and Kretschmann (1989) reported an average ratio of 0.80 with a range of 0.78 to

0.83 for three major species groups (Douglas Fir-Larch, Hem-Fir and Southern Pine). The average ratio for all species was 0.83.

Fifth percentile of MOE E0,05 is used in calculations where member stiffness

takes direct influence on member strength, e. g. overall structural stability, buckling and lateral torsional stability. EN 384 and EN 338 assume a constant ratio of fifth percentile (E0,05) and mean value (E0,mean) of MOE (Table1):

E0;05=E0;mean¼ 0:67 for softwood species ð3Þ For infinite sized normally distributed samples, this fractile ratio corresponds to a

COV of 20%. Green and Kretschmann (1989) suggested to lower the ratio and to

make it a function of strength class.

Ratio of MOE in bending, tension and compression parallel to the grain

Most investigations on the ratio between the moduli of elasticity were carried out

with small clear specimens (Conners and Medvecz1992). Clear specimens exhibit

identical tensile and compression MOE (Thunell1941). Garfinkel (1973) developed

his wooden beam analysis on the assumption that the ratio of tension MOE to

compression MOE is between 1.00 and 1.05. Kollmann and Coˆte´ (1968) expected

the ratio to be approximately 1.00 for softwood. For sugar maple and basswood,

Schneider and Phillips (1991) found different parallel-to-the-grain MOE values in

bending, tension and compression. Burger and Glos (1995) showed that the MOE in

tension and in bending of full-size spruce structural timber, in contrast to small clear specimens, depends on the type of load as well as on timber quality. The authors

evaluated test results of 147 European spruce specimens dimensioned 50/120 mm2

(54 specimens) and 60/105 mm2(93 specimens). On average, bending MOE Emwas

9% higher than the tensile MOE Et and the following regression Eq. (4) was

reported:

Em¼ 90 þ 1:077Et N=mm2

with R¼ 0:94 ð4Þ

EN 338 does not make any difference in MOE depending on the type of loading

(bending, tension, compression) and gives one single value E0 (Table 1). If the

differences between Em, Etand Ecfor timber in structural sizes actually are small,

assigning one single MOE value is a good solution, since the process of designing timber structures can be kept simple.

Aim of the study

Correct property relationships are very important for the design of economic and reliable timber structures. The objective of this study was to review some of these property relationships based on recently compiled large data sets as a contribution for a future revision of the grading standards. Based on several series of tests with Norway spruce structural timber, the following property relationships were analysed:

• relationship of bending strength and bending MOE,

• simultaneous matching of in-grade basic characteristic values MOR fm,k, mean

MOE (derived from bending tests) E0,meanand density rk,

• ratio of characteristic tensile and compression strength parallel to the grain ft,0,k

and fc,0,kto characteristic bending strength fm,k,

• ratio of 5th-percentiles and mean values of density r and MOE E0,

Materials and methods Data sets

Three data sets from different extensive research projects, referenced (1) to (3) served as data base:

1. In the early 1990s a test program was launched at the ETH Zurich, which aimed

to evaluate the mechanical properties of Swiss grown Norway spruce structural timber (Steiger1995a,b,1996).

2. The second source of data is a research project started after the extraordinarily violent winter storm ‘Lothar’ in Central Europe in December 1999, aiming at collecting more information regarding the extent and location, the causes, the detection, and the consequences of wind-induced compression failures (Arnold and Steiger2007). Property relationship analysis of this data source, however, was only carried out using data resulting from reference tests on samples without any storm damages.

3. A third source of data is a Ph.D. thesis (Mischler-Schrepfer2000) dealing with

the influence of long-term log storage in the forest on the mechanical properties of timber.

In order to get large sample sizes, the data taken from the above mentioned studies were pooled for the different analysis steps (Tables2,3,4):

(A) Data set (A) (Table2) consisted of bending test data (MOE Emand MOR fm) of

696 specimens of cross-section b/h (mm): 60/120, 80/160, 100/160 and 95/110. (B) In data set (B) (Table 3) results from 796 tension tests (MOE Et,0and tension

strength ft,0) were pooled. The dimensions of the specimens covered a broad

range from plank-type specimens to squared timber.

(C) Due to the fact that compression tests were not treated with the same priority

within project (1), the compression data pool (C) (Table 4) was smaller

(ntot= 152) than data sets (A) and (B). However, since variation of test values

is smaller compared to the tension and bending tests, this is no problem for the data analysis.

Table 2 Data pool (A): specimens tested in edgewise bending (see Fig.2a) Source Cross-section

b/h (mm)

Sample size n

Span ‘ (mm) Distance between loading points ‘ - 2a (mm) Gauge length ‘1(mm) 1 60/120 53 2,160 = 18h 720 = 6h 500 = 4.17h 80/160 and 100/160 244a 2,700 = 16.88h 900 = 5.62h 600 = 3.75h 80/160 36 2,760 = 17.25h 920 = 5.75h 600 = 3.75h 2 95/110 363 1,980 = 18h 660 = 6h 550 = 5h ntot 696 EN 408 specifications 18h 6h 5h a

(D) The data needed for the comparison of MOE in bending, tension and compression were collected in the course of interaction tests on 80/160 mm beams simultaneously loaded by a bending moment and a normal (tension or

compression) force (Steiger and Fontana 2005) being part of project (1)

(Steiger1995b). Sample size amounted to 109 pairs of values (Em; Et) and 81

pairs of values (Em; Ec). All specimens were cut according to the sawing

pattern shown in Fig.1.

Table 3 Data pool (B): specimens tested in tension parallel to the grain (see Fig.2b)

Source Cross-section b/h (mm) Sample size n Free length ‘F(mm) Gauge length ‘M(mm)

1 10/180 7 910–1,220 = 5.06–6.78h 900 = 5h 20/180 21 1,640 = 9.11h 900 = 5h 30/180 50 1,640 = 9.11h 900 = 5h 40/180 21 1,640 = 9.11h 900 = 5h 30/150 34 1,620 = 10.80h 900 = 6h 80/80 40 1,200 = 15h 900 = 11.25h 80/120 46 1,200 = 10h 900 = 7.50h 80/160 19 1,100 = 6.88h 900 = 5.63h 80/180 21 1,200 = 6.67h 900 = 5h 60/180 42 1,200 = 6.67h 900 = 5h 2 45/150 104 4,300 = 28.67h 750 = 5h 3 29/150 126 3,300 = 22h 750 = 5h 45/150 156 3,300 = 22h 750 = 5h 49/150 109 3,300 = 22h 750 = 5h ntot 796 EN 408 specifications 9h 5h

Table 4 Data pool (C): specimens tested in compression parallel to the grain (see Fig.2c) Source Cross-section b/h (mm) Sample size n Length ‘ (mm) Free length 0.5‘ (mm) Gauge length ‘M(mm) 1 60/120 46 1,000 = 8.33h 500 = 8.33b 600 = 10b 80/160 19 1,500 = 9.38h 750 = 9.38b 900 = 11.25b 100/160 40 1,500 = 9.38h 750 = 7.50b 900 = 9b 140/240 47 1,500 = 6.25h 750 = 5.36b 700 = 5b ntot 152 EN 408 specifications: – 6b 4b

Test procedures

All three studies (1)–(3) used similar test procedures (Tables2,3,4). Testing was

carried out in accordance with EN 408 (2003) and the characteristic values were

determined according to EN 384 (2004). The critical section was always positioned

in such way that it was subjected to maximum load.

Moisture content was measured by the electric resistance method. Density was determined from the mass and the volume of the whole specimen. The ‘‘global’’ density values were adjusted to the density of small defect-free prisms (ISO 3131

1975) by dividing by 1.05 given in EN 384.

Tests to derive bending MOE and bending strength were performed in edgewise position. The tension edge was selected at random. The test pieces, having a minimum length of approximately 19 times the depth of the section, were simply supported and symmetrically loaded in bending at two points over a span of approximately 18 times the depth. MOE was measured within the loading points. In the course of project (1), the concept of proof loading with a threshold of 40 N/mm2 was used, resulting in 214 values of bending MOE but in only 88 bending strength

values. With respect to notations in Fig.2a and d, Table2 lists geometrical

properties of bending tests carried out.

Tension tests parallel to the grain were carried out according to EN 408, the

timber being of full cross-section (Fig.2d). Geometrical properties of specimens

subjected to tension tests are presented in Table3 with notations according to

Fig. 1 Sawing pattern of
interaction test specimens
(80/160 mm)
a = 6h ± 1.5h 6h
l1 = 5h
δ
l = 18h ± 3h
h
h/2 h/2
F/2
F/2
a = 6h ± 1.5h
**(a)**
b
h
** (d) **
*h = height or depth *
*b = width *
lV
lE
l
lM lF
lE
lV
**(b)**
0.5l
l
0.5l
lM
**(c)**

Fig. 2 Test configurations to perform bending (a) and parallel-to-the-grain tension (b) and compression tests (c). All specimens were of rectangular cross-section b/h (d)

Fig.2b. Tests were carried out with special test equipment set up and optimised based on preliminary studies presented in (Steiger et al.1994).

Compression tests were carried out with lateral restraints at half-length to prevent

the specimens from buckling (Fig.2c). Geometrical properties of the specimens are

listed in Table4.

Assessment of timber quality

The MOE, although not being a direct parameter to define strength, but depending

on the same factors, is the best single indicator of timber quality (Glos 1995).

Instead of the static MOE, dynamic MOE Edynwas used as a reference indicator of

quality. Edynwas calculated from the velocity v of an ultrasonic wave passing the

specimen longitudinally and from the specimen’s density r [Eq. (5)]. Such

measurements, originally described by Goens (1931), are successfully used for

assessing the quality of structural timber (Hearmon 1966; Kollmann and Krech

1960).

Edyn¼ rv2 ð5Þ

Equation (5) is valid if the wave length is bigger than the lateral dimensions of the specimens. For Norway spruce timber typical ultrasonic wave velocities are in the range of 5,000–6,000 m/s, resulting in wave lengths between approximately 15 and 40 cm.

The longitudinal ultrasonic wave velocity was determined from specimen length and travel time of the signal. The ultrasonic testers Steinkamp BP V (fre-quency = 50 kHz) and Sylvatest (fre(fre-quency = 16 kHz) were used. To account for the influence of moisture on the ultrasonic wave velocity, Eq. (6) (Sandoz1990) and (7) were used. Equation (7) is a linearization of (6), which for different MCs (MC1,

MC2) between 10 and 20% is equal to Eq. (6).

v1¼ v2 1 0:0053 MC2 MC1ð Þ ½ for MC \ 28% ð6Þ v1 ¼ v2þ 29 MC2 MC1ð Þ for MC \ 28% ð7Þ Data processing

According to EN 384, characteristic values (sample fifth percentiles) are to be estimated by determining the fifth percentiles of ranked samples. However, with regard to in-grade samples of usually smaller size, the analysis to calculate fifth percentiles used parametric methods to take into account all the information provided by the test results. In case of strength variables, a lognormal distribution was used. MOE and density data were analysed assuming normal distributions.

Dynamic MOE Edynwas used to group test values according to timber quality.

Grouping always aimed to get at least 40 specimens in each group. Usually, groups contained more than 60–80 specimens.

According to EN 384, the reference wood moisture content shall be consistent with 20C and 65% relative humidity, which for most softwood corresponds to a

MC of about 12%. For samples not tested at reference conditions but having a mean MC in the range of 10 to 18%, adjustment of lower fifth percentile or mean values to 12% MC was made according to EN 384 as follows:

• for bending and tensile strength: no adjustment

• for compression parallel to the grain strength: 3% change for every percentage

point difference in MC

• for MOE: 2% change for every percentage point difference in MC

The adjustments were carried out in a way that the above-quoted properties increase if the data are adjusted from a higher MC, and vice versa.

For bending strength, the reference dimensions correspond to a depth (height) h of 150 mm and to the standard test set-up proportions of four point bending with loads applied in the third points and an overall span of 18 times the specimen depth h. Tensile strength is given for a reference width h of 150 mm. For samples not tested at reference conditions, EN 384 gives adjustment factors. Size adjustment to 150 mm depth or width can be made by dividing the fifth percentile by kh [Eq. (8)]: kh¼ 150 h 0:2 ð8Þ

Tensile strength data resulting from tests with different lengths ‘et can be

adjusted to reference length ‘esby using Eq. (9) with an exponent of m‘ = 0.15. k‘¼

‘es ‘et

m‘

ð9Þ

Results and discussion Timber quality

Dynamic MOE Edyn, which can be measured non-destructively, is a good

indicator of actual stiffness (MOE) and strength of timber in bending, tension

and compression as shown in Fig.3. Figures3a–c confirm a strong correlation

(R = 0.77–0.90) between static and dynamic MOE. Hence, it can be concluded that MOE can be derived by a much simpler dynamic measurement together with density instead of carrying out static bending tests. Regarding machine grading, dynamically measuring MOE provides the only possibility of grading timber members with thickness of more than 75 mm, since most stress grading machines with static MOE measurements are limited to member thicknesses up to 75 mm.

According to Fig.3d–f the correlation between dynamic MOE and bending,

parallel-to-the-grain compression and tensile strength is weaker (R = 0.59–0.72). However, the correlation still is strong enough to use dynamic MOE as one of the indicators for timber strength when equipping grading machines or when assigning experimental data to given strength classes.

Relationship of bending strength and bending MOE

The correlation between bending strength fm and bending MOE Emderived from

static bending tests is shown in Fig.4. The coefficient of correlation amounts to

*y = 0.8586x - 1357*
*R = 0.77 (R*2
= 0.60)
*n = 668*
0
5000
10000
15000
20000
25000

**Dynamic MOE E****dyn**** [N/mm**

**2 _{]}**

**Dynamic MOE E****dyn**** [N/mm2]**

**Dynamic MOE E****dyn**** [N/mm**

**2**

**]** **Dynamic MOE E****dyn**** [N/mm**

**2**
**]**
**Dynamic MOE E****dyn**** [N/mm**

**2 _{]}**

**Stat**

**ic**

**M**

**O**

**E in**

**bending**

**E****m****[**

**N**

**/m**

**m**

**2]**

**(a)**

*y = 0.0034x - 5.25*

*R = 0.62 (R*2 = 0.39)

*n = 522*0 10 20 30 40 50 60 70 80 90 100

**Be**

**nding st**

**re**

**n**

**gt**

**h**

**f****m****[N**

**/m**

**m**

**2]**

**(d)**

*y = 0.9539x - 2483*

*R = 0.90 (R*2

_{ = 0.80)}

*n = 771*0 5000 10000 15000 20000 25000

**S**

**tat**

**ic**

**M**

**O**

**E in t**

**en**

**si**

**on**

**E****t,0****[N**

**/mm**

**2]**

**(b)**

*y = 0.0027x - 11.1*

*R = 0.59 (R*2 = 0.34)

*n = 796*0 10 20 30 40 50 60 70 80 90 100

**Tension strength**

**f****t,0****[N/**

**mm**

**2]**

**(e)**

*y = 0.9353x - 3104*

*R = 0.84 (R*2 = 0.70)

*n = 167*0 5000 10000 15000 20000 25000

**S**

**tatic MOE i**

**n**

**comp**

**ress**

**ion**

**E****c,**

**0****[N/**

**m**

**m**

**2]**

**(c)**

*y = 0.002x - 2.08*

*R = 0.72 (R*2 = 0.52)

*n = 167*0 10 20 30 40 50 60 70 80 90 100 0

**C**

**o**

**m**

**p**

**re**

**ss**

**io**

**n**

**s**

**tr**

**en**

**gt**

**h**

**f****c,0****[N**

**/m**

**m**

**2]**

**(f)**

**Dynamic MOE E****dyn**** [N/mm**

**2 _{]}**
25000
20000
15000
10000
5000
0 5000 10000 15000 20000 25000 0 5000 10000 15000 20000 25000
0 5000 10000 15000 20000 25000
0 5000 10000 15000 20000 25000 0 5000 10000 15000 20000 25000

Fig. 3 Correlation of dynamic MOE Edynwith MOE in bending Em(a), tension Et,0(b), compression Ec,0 (c) and with bending strength fm(d), tensile strength ft,0(e) and compression strength fc,0(f)

R = 0.66, which is lower compared to other studies reported in Glos (1995). The EN 338 basic strength class values (characteristic bending strength fm,kand MOE parallel

to the grain E0,mean) follow the trend of the experimental data up to strength class C24

(fm,k= 24 N/mm2). In strength classes C27–C50 (fm,k= 27 to 50 N/mm2), the

bending MOE found in our tests is higher than the assigned strength class value. The reason for this is not clear and no answer could be found in background documents of the standard and in the corresponding literature. Assigning lower MOE in strength classes for high-performance timber might, however, be a hidden additional safety intended by the responsible standardisation committee.

Simultaneous matching of in-grade basic characteristic values of MOR, mean MOE and density

In order to assign a sample to a certain strength class provided by EN 338, the characteristic values (fifth percentiles) of bending strength fm,k and density rk as

well as the mean MOE parallel to the grain E0,meanhave to match or exceed the

class values. The data set derived from bending tests (sample size n = 522) was

divided into six equally sized groups according to measured dynamic MOE Edyn.

The above-mentioned characteristic values were calculated for each group and

compared to the code values given in EN 338. Figure5 shows that the test data

match the strength class profile given by EN 338 very well. For strength classes

with MOE [13,000 N/mm2 the tests exhibit somewhat higher MOE values than

assigned by EN 338. Hence, based on the tests results described in this study, there is no reason for changing in-grade discrimination of basic characteristic values fm,k, E0,meanand rk.

*y = 0.003x + 10.6*
*R = 0.66 (R2* = 0.43)
*n = 525*
0.0
10.0
20.0
30.0
40.0
50.0
60.0
70.0
80.0
90.0
0
**Bending MOE ****E****m**** [N/mm2]**
**B**
**en**
**d**
**in**
**g s**
**tr**
**engt**
**h**
** **
**f****m**** [N**
**/m**
**m**
**2** **]**
Regression line
lower 5% confidence limit

+ Test values

EN 338 strength class values

*fm ,k and E0,m ean*
20000
18000
16000
14000
12000
10000
8000
6000
4000
2000

Fig. 4 Bending strength fmversus bending MOE Emderived by static tests (edgewise). The dots indicate pairs of (fm,k; E0,mean) given in EN 338 (Table1)

Ratio of tensile and compression strength parallel to the grain to bending strength

A direct comparison of bending and tensile or compression strength is not possible since one cannot test the same specimen to failure in bending and in tension or compression, respectively. The ratio of characteristic values of tensile strength ft,0,k

to bending strength fm,kshown in Fig.6a was therefore derived from data grouped

according to the dynamic MOE Edynwith equal class boundaries for both bending

and tensile strength data sets (five groups). The relationship of tensile and bending

strength on the mean as well as on the fifth percentile level is shown in Fig.6b

together with linear trend lines. The ratio of tensile to bending strength obviously is not constant but rather depends on timber quality. Ratios of mean values and characteristic values exhibit the same trend. Assuming a constant ratio of ft/fm= 0.6

according to Eq. (1) gives safe results for characteristic bending strength values

fm,kC 22 N/mm2(EN 338 strength classes C22 and higher). For fm,k\ 22 N/mm2,

however, the ratio derived from the test results is smaller than 0.6. Hence, it is suggested to analyse other data sets, in order to get reliable information on ratios of tensile to bending strength for strength classes lower than C22.

The ratio of characteristic values of compression strength fc,0,kto bending strength

fm,kshown in Fig.7a was derived from data grouped again according to the dynamic

MOE Edynwith equal class boundaries for both bending and compression strength

data sets (four groups). The relationship of compression and bending strength on the mean as well as on the fifth percentile level is shown in Fig.7b together with power

trend lines. Compared to our test results the EN approach [Eq. (2)] is more

conservative for characteristic bending strength values fm,kC 24 N/mm

2

(EN 338 strength classes C C24). The trend line fitting the test results progresses equally on the mean and on the characteristic level. An extrapolation of the trend to

0.0
10.0
20.0
30.0
40.0
50.0
60.0
70.0
80.0
90.0
100.0
0
**Bending MOE E****m**** [N/mm**
**2**
**]**
**Char. **

**value of bending strength **

** f****m,****k**** [N/mm**
**2** **]**
0
50
100
150
200
250
300
350
400
450
500
**C**
**h**
**aracteristic **
**value of density **
** r****k****[kg/m**
**3]**

fm,k test values with linear trend line fm,k EN 338 values

rk test values with linear trend line rk EN 338 values 20000 18000 16000 14000 12000 10000 8000 6000 4000 2000

Fig. 5 Comparison of EN 338 basic strength class values fm,k, E0,meanand rk(Table1) and test values (with linear trend lines)

characteristic bending strengths fm,k\ 24 N/mm2, however, results in lower fc,0,k

values compared to the characteristic values assigned by Eq. (2) and thus Eq. (2) overestimates fc,0,kin strength classes lower than C24.

EN 338 values as well as test values (four groups graded according to Edyn)

exhibit a linear relationship between the compression strength parallel to the grain fc,0and the wood density r (Fig.8). The slope of the regression line found in our

tests, however, is almost twice the slope of the trend line fitted to the code values. This confirms again the overestimation of fc,0,kby Eq. (2) for fc,0,k\ 20 N/mm2. As

an alternative to the code approach [Eq. (2)], the compression strength parallel to the grain could be derived from the wood density using a linear model.

Ratio of fifth percentile and mean value of density and MOE

The ratio between characteristic and mean value of density (MC = 12%) of all

1,640 specimens results in rk/rmean= 0.84. The mean value is 450 kg/m3and the

0.0
0.1
0.2
0.3
0.4
0.5
0.6
0.7
0.8
0.9
1.0
20
**Bending strength f****m,k**** [N/mm**
**2 _{]}**

**Ra**

**ti**

**o**

**f****t**

**/f****m**Test values with linear trend line: char. level
Test values with linear trend line: mean level
EN 338: ft,k/fm,k = 0.6
*(1) y = 0.86x - 5.80; R2*
= 0.97
*(2) y = 1.11x - 13.3; R2*
= 0.97
5
10
15
20
25
30
35
40
45
50
55
60
**Bending strength f****m,k**** [N/mm**
**2 _{]}**

**T**

**ens**

**il**

**e stre**

**ngth**

**f****t,****0,k****[N/mm**

**2]**

Test values with linear trend line (1): char. level
Test values with linear trend line (2): mean level
EN 338: ft,k = 0.6 fm,k
60
55
50
45
40
35
30
25 20 25 30 35 40 45 50 55 60
**(a)** **(b)**

Fig. 6 Ratio (a) and relationship (b) of bending strength fmand tensile strength ft

*(2) y = 2.56x*-0.34*; R2* = 0.88
*(1) y = 2.65x*-0.35*; R2* = 0.93
0.0
0.1
0.2
0.3
0.4
0.5
0.6
0.7
0.8
0.9
1.0
**Ra**
**ti**
**o **
**f****c****/f****m***EN 338: fc,0,k/fm,k = 5(fm,k*)
-0.55

Test values with power trend line(1): char. level Test values with power trend line (2): mean level

*(2) y = 2.56x*0.66
*; R2*
= 0.96
*(1) y = 2.65x*0.65*; R2* = 0.98
10
15
20
25
30
35
40
20 30 40 50 60
20 30 40 50 60
**Bending strength f****m,k**** [N/mm**
**2**
**]**
**Bending strength f****m,k**** [N/mm**
**2 _{]}**

**Co**

**mp**

**ressio**

**n stren**

**gth**

**f****c,****0,k****[N/**

**m**

**m**

**2]**

*EN 338: fc,0,k = 5(fm,k*) 0.45

Test values with power trend line (1): char. Test values with power trend line (2): mean

**(a)** **(b)**

COV amounts to approximately 9.7%. The normal probability plot (Fig.9a) confirms the assumption of a normal distribution for density. The test results are in

line with the code procedures of EN 338 and EN 384 (COV = 10% and ratio rk/

rmean = 0.84).

The ratio of characteristic to mean MOE calculated based on all results of

bending tests (n = 668) yields in E05/Emean= 0.70. The COV is 18.4% and a

normal distribution fits the data reasonably well (Fig.9b). These results confirm the ratio and COV given in EN 338 and EN 384, which are 0.67 and 20%, respectively.

*(3) y = 0.077x - 6.46; R*2 = 0.99
*(2) y = 0.13x - 22.8; R2* = 0.96
*(1) y = 0.14x - 30.6; R2* = 0.98
0.0
5.0
10.0
15.0
20.0
25.0
30.0
35.0
40.0
200 300 400 500 600
**Wood density r [kg/m****3]**
**Co**
**mp**
**ress**
**ion**
** stren**
**g**
**th**
** **
**f****c,****0**** [N/mm**
**2** **]**

Test values with linear trend line (1): char. level Test values with linear trend line (2): mean level EN 338 values with linear trend line (3)

Fig. 8 Relationship between compression strength parallel to the grain fc,0and wood density r: Test results and EN 338 values (Table1)

250 300 350 400 450 500 550 600 650
.01
.1
1
5
10
20
30
50
70
80
90
95
99
99.9
99.99
**Density r [kg/m****3]**
[%]
n = 1640
Min = 321 kg/m3
Max = 623 kg/m3
Mean = 450 kg/m3
Stdev = 43.5 kg/m3
COV = 9.68%
r
k = 378 kg/m
3
r
k/rmean = 0.84
5000 10000 15000 20000
.01
.1
1
5
10
20
30
50
70
80
90
95
99
99.9
99.99
**MOE in bending E**_{m}** [N/mm2]**
[%]
n = 668
Minimum = 4823 N/mm2
Maximum = 19226 N/mm2
Mean = 13111 N/mm2
Stdev = 2409 N/mm2
COV = 18.4%
E
05 = 9150 N/mm
2
E
05/Emean = 0.70
**(a)** **(b)**

Ratio of MOE in bending, tension and compression

The relationships of bending MOE Emand tensile MOE Etor compression MOE Ec

are shown in Fig.10. The following linear regression Eqs. (10) and (11) could be

derived from the tests:

Et¼ 0:808Em 2;523 with R¼ 0:91 R2¼ 0:83 ð10Þ Ec¼ 0:745Emþ 3;357 with R¼ 0:85 R2¼ 0:72 ð11Þ

Based on Eqs. (10) and (11), MOE values Et and Ec and ratios Et/Em and

Ec/Em were calculated and compared to MOE values given in EN 338 for the

whole strength class spectrum C14 to C50 (Table5). Furthermore, the MOE

ratios are plotted in Fig.11. On average, bending MOE derived according to the

EN 408 4-point bending test differed only by 1% from MOE in tension or in compression. However, the ratios are not constant; they depend on the timber quality:

• low-quality timber (for example class C18): Et=Em¼ 1:09 Ec=Em¼ 1:12

• normal-quality timber of classes C24–C30: Et=Em¼ 1:03 Ec=Em¼ 1:04

• high-quality timber of classes C35 and C40: Et=Em¼ 1:00 Ec=Em¼ 1:00:

Timber members assigned to classes C35 and C40 are free of defects. That is why such members behave similar to small clear specimens resulting in identical MOE Et, Ec, Em.

Looking at the process of designing timber structures, the practice of EN 338 of
giving one single MOE value for each strength class is a good approach. However,
when grading timber based on tension MOE instead of bending MOE, the
differences reported above have to be taken into account. Then, timber has to be
modelled as a composite material with zones of different MOE within cross-section
(Gehri1997).
*y = 0.808 x + 2523*
*R = 0.91; R*2
= 0.83
*n = 109*
5000
10000
15000
20000
25000
5000
**MOE in bending E****m**** [N/mm**
**2**
**]**
**M**
**O**
**E in**
** t**
**ension **
**E****t****[N/**
**m**
**m**
**2]**
**M**
**O**
**E**
** i**
**n**
** compression **
**E****c****[N/**
**mm**
**2]**
*y = 0.745 x + 3357*
*R = 0.85; R*2
= 0.72
*n = 81*
5000
10000
15000
20000
25000
5000
**MOE in bending E****m**** [N/mm**
**2**
**]**
25000
20000
15000
10000
25000
20000
15000
10000
**(a)** **(b)**

Fig. 10 Bending MOE Emversus MOE in tension Et(a) and in compression Ec(b) for Norway Spruce structural timber with cross-section 80/160 mm

Conclusion

Our investigations lead to the following conclusions:

• Overall, the test results in this study confirm the property relationships and

strength class profiles regarding bending strength, tension strength, compression strength, density and MOE given in EN 338. No reasons for substantial changes of these values were found.

Table 5 Ratios of bending MOE Emand MOE in tension Etor in compression Ecfor Norway spruce solid timber with cross-section 80/160 mm

Strength class Em(N/mm2) acc. to EN 338

Et(N/mm2) calc. with Eq. (10)

Ec(N/mm2) calc. with Eq. (11)

Ratio Et/Em Ratio Ec/Em

C14 7,000 8,200 8,600 1.17 1.23 C16 8,000 9,000 9,400 1.13 1.18 C18 9,000 9,800 10,100 1.09 1.12 C20 9,500 10,200 10,500 1.07 1.11 C22 10,000 10,600 10,900 1.06 1.09 C24 11,000 11,400 11,600 1.04 1.06 C27 11,500 11,800 12,000 1.03 1.05 C30 12,000 12,200 12,400 1.02 1.03 C35 13,000 13,000 13,100 1.00 1.01 C40 14,000 13,900 13,900 0.99 0.99 C45 15,000 14,700 14,600 0.98 0.97 C50 16,000 15,500 15,400 0.97 0.96

Italic, extrapolation; bold, normal-quality timber

0.80
0.90
1.00
1.10
1.20
1.30
6000 7000 8000 9000 10000 11000 12000 13000 14000 15000 16000
**MOE in bending E****m**** [N/mm**
**2**
**]**
**M**
**O**
**E**
** r**
**a**
**tio**
** E****t,****0****/E****m**** or**
** E****c,0****/E*** m* Ratio Ec,0/Em
Ratio Et,0/Em

**C1**

**6**

**C2**

**4**

**C3**

**0**

**C4**

**0**

• The good correlation between dynamic MOE and static MOE (bending, tension, compression) as well as strength (MOR, tension and compression parallel to the grain) recommends using ultrasonic wave speed together with density as an indicator of timber quality.

• The coefficient of correlation of bending strength and bending MOE derived

from static bending tests amounts to R = 0.66 and is consistent with other studies and confirms limitation of strength prediction.

• Tensile to bending strength ratio was found not to be constant, but to depend on

timber quality. Ratios for characteristic bending strengths fm,kC 22 N/mm2(EN

338 classes above C22) amounted to 0.6–0.75 but were \ 0.6 for lower quality timber.

• The relationship between the characteristic values of compression and bending

strength parallel to the grain given in EN 384 [Eq. (2)] is more conservative for higher quality timber than our test results indicate. As an alternative to the existing approach, the compression strength parallel to the grain could be derived from wood density using a linear model. Doing so, the importance of density as a classification criterion would be increased.

• The calculated fractile ratios for density rk/rmean and for MOE parallel to the

grain E0,05/E0,mean were 0.84 and 0.70. These values correspond well to the

ratios given in EN 384 and EN 338 (0.84 and 0.67) assuming a COV of 10% and 20%, respectively.

• The ratios of MOE of Norway spruce structural timber with a cross-section of

80/160 mm in tension, compression and bending differ depending on timber quality. Differences up to 9% between tensile and bending MOE were found. Regarding compression MOE, the maximum difference to the bending MOE was 12%. For normal-quality timber of classes C24–C30 (mainly used in

practice), the differences between Et, Ec and Emare not more than 6%. With

regard to a simple design process, the current practice of using one single MOE value should therefore not be changed. However, when assigning timber populations to strength classes based on tension MOE instead of bending MOE, the differences have to be taken into account. In this case, timber must be regarded as a composite material having zones of different MOE within cross-section.

References

Arnold M, Steiger R (2007) The influence of wind-induced compression failures on the mechanical properties of spruce structural timber. Mater Struct 40(1):57–68

Burger N, Glos P (1995) Relationship of moduli of elasticity in tension and in bending of solid timber. Paper 28-5-2. In: Proceedings of CIB-W18 Meeting 28, April 1995, Copenhagen, Denmark Burger N, Glos P (1997) Strength relationships in structural timber subjected to bending and tension.

Paper 30-6-1. In: Proceedings of CIB-W18 Meeting 30, August 1997, Vancouver, Canada Conners TE, Medvecz PJ (1992) Wood as a bimodular material. Wood Fiber Sci 24(4):413–423

Curry WT, Fewell AR (1977) The relations between the ultimate tension and ultimate compression strength of timber and its modulus of elasticity. Research Report CP22/77, Princes Risborough Laboratory, Building Research Establishment BRE, Buckinghamshire

Ehlbeck J, Werner H (1992) Coniferous and deciduous embedding strength for dowel-type fasteners. Paper 25-7-2. in: Proceedings of CIB-W18 Meeting 25, August 1992, A˚ hus, Sweden

EN 338 (2003) Structural timber–strength classes. Comite´ Europe´en de Normalisation CEN

EN 408 (2003) Timber structures—structural timber and glued laminated timber—determination of some physical and mechanical properties. Comite´ Europe´en de Normalisation CEN

EN 384 (2004) Structural timber : determination of characteristic values of mechanical properties and density. Comite´ Europe´en de Normalisation CEN

Fewell AR (1982) Machine Stress Grading of Timber in the United-Kingdom. Holz Roh Werkst 40(12):455–459

Garfinkel G (1973) Wood engineering. Southern Forest Products Association, New Orleans

Gehri E (1997) Timber as a natural composite: Explanation of some peculiarities in the mechanical behaviour. Paper 30-6-3. in: Proceedings of CIB-W18 Meeting 30, August 1997, Vancouver, Canada

Gindl W, Teischinger A (2002) Axial compression strength of Norway spruce related to structural variability and lignin content. Composites Part a. Appl Sci Manufact 33(12):1623–1628

Glos P (1995) Step A6: Festigkeitssortierung. In: Holzbauwerke nach Eurocode 5, Step 1: Bemessung und Baustoffe, Informationsdienst Holz. Arbeitsgemeinschaft Holz e. V, Du¨sseldorf, Germany Goens E (1931) The determination of the elasticity module of rods with the help of bending fluctuations.

Annalen der Physik 11(6):649–678

Green DW, Kretschmann DE (1989) A discussion of lumber property relationships in Eurocode 5. Paper 22-6-3. In: Proceedings of CIB-W18 Meeting 22, September 1989, Berlin, German Democratic Republic

Green DW, Kretschmann DE (1990) Stress class systems: an idea whose time has come? Research Paper FPL-RP-500. Forest Products Laboratory, Madison

Hearmon RFS (1966) Vibration testing of wood. Forest Prod J 16(8):29–40

ISO 3131 (1975) Wood; Determination of density for physical and mechanical tests. International organization for standardization

Kollmann F, Krech H (1960) Dynamische Messung der elastischen Holzeigenschaften und der Da¨mpfung. Holz Roh-Werkst 18(2):41–54

Kollmann FFP, Coˆte´ WA Jr (1968) Principles of wood science and technology, vol 1: solid wood. Springer, Berlin

Mischler-Schrepfer V (2000) Der Einfluss der Waldlagerung von Fichten-Rundholz auf die La¨ngs-Zugeigenschaften des Schnittholzes, Ph.D. thesis, ETH Zu¨rich, Switzerland

Ruli A (2004) Determination of the compression strength of glulam - longitudinal and perpendicular to the grain. Diploma thesis, Institute of Timber Engineering and Wood Technology, Graz University of Technology, Austria

Sandoz J-L (1990) Triage et fiabilite´ des bois de construction validite´ de la me´thode ultrason, Lausanne, Ph.D. thesis, EPF Lausanne, Switzerland

Schneider MH, Phillips JG (1991) Elasticity of wood and wood polymer composites in tension, compression and bending. Wood Sci Technol 25(5):361–364

Steiger R (1995a) Biege-, Zug- und Druckversuche an Schweizer Fichtenholz, Institut fu¨r Baustatik und Konstruktion, ETH Zu¨rich, Research Report Nr. 207, Birkha¨user Verlag, Basel, Switzerland Steiger R (1995b) Versuche an Fichten-Kantho¨lzern: Biegemoment-Normalkraft-Interaktion, Institut fu¨r

Baustatik und Konstruktion, ETH Zu¨rich, Research Report Nr. 209, Birkha¨user Verlag, Basel, Switzerland

Steiger R (1996) Mechanische Eigenschaften von Schweizer Fichten-Bauholz bei Biege-, Zug-, Druck-und kombinierter M/N-Beanspruchung, Research Report Nr. 221, Birkha¨user Verlag, Basel, Switzerland

Steiger R, Arm H, Gehri E (1994) Einspannvorrichtung fu¨r Zugversuche an Holzproben gro¨sseren Querschnitts, Institut fu¨r Baustatik und Konstruktion, ETH Zu¨rich, Research Report Nr. 204, Birkha¨user Verlag, Basel, Switzerland

Steiger R, Fontana M (2005) Bending moment and axial force interacting on solid timber beams. Mater Struct 38(279):507–513

Thelandersson S (1995) Step 3/11: Deformations in timber structures. In: Holzbauwerke nach Eurocode 5, Step 3: Grundlagen, Entwicklungen, Erga¨nzungen, Informationsdienst Holz. Arbeitsgemeinschaft Holz e. V, Du¨sseldorf

Thunell B (1941) U¨ ber die Elastizita¨t schwedischen Kiefernholzes. Holz Roh- Werkst 4(1):15–18 Ylinen A (1942) U¨ ber den Einfluss des Spa¨tholzanteiles und der Rohwichte auf die Festigkeits- und

elastischen Eigenschaften des Nadelholzes. Acta forest. Fenn. 5:1. Cited In: Kollmann FFP, Coˆte´ Jr. WA (Ed.): Principles of Wood Science and Technology, vol 1: Solid Wood, Springer, Berlin, 1968, pp 346